Approaches to Overcome Nodules and Scratches on Wire Bondable Plating on
Young K. Song and Vanja Bukva, Teledyne DALSA Inc., Waterloo, ON, Canada
Ryan Wong, FTG Circuits, Toronto, ON, Canada
Initially adopted internal specifications for acceptance of printed circuit boards (PCBs) used for wire bonding was that there
were no nodules or scratches allowed on the wire bond pads when inspected under 20X magnification. The nodules and
scratches were not defined by measurable dimensions and were considered to be unacceptable if there was any sign of a
visual blemish on wire bondable features. Analysis of the yield at a PCB manufacturer monitored monthly for over two years
indicated that the target yield could not be achieved, and the main reasons for yield loss was due to nodules and scratches on
the wire bonding pads.
The PCB manufacturer attempted to eliminate nodules and scratches. First, a light scrubbing step was added after electroless
copper plating to remove any co-deposited fine particles that acted as a seed for nodules at the time of copper plating. Then
the electrolytic copper plating tank was emptied, fully cleaned, and filtered to eliminate the possibility of co-deposited
particles in the electroplating process. Both actions greatly reduced the density of the nodules but did not fully eliminate them.
Even though there was only one nodule on any wire bonding pad, the board was still considered a reject. In order to reduce
scratches on wire bonding pads, the PCB manufacturer utilized foam trays after routing the boards so that they did not make
direct contact with other boards. This action significantly reduced the scratches on wire bonding pads, even though some
isolated scratches still appeared from time to time, which caused the boards to be rejected. Even with these significant
improvements, the target yield remained unachievable.
Another approach was then taken to consider if wire bonding could be successfully performed over nodules and scratches,
and if there was a dimensional threshold where wire bonding could be successful. A gold ball bonding process called either
stand-off-stitch bonding (SSB) or ball-stitch-on-ball bonding (BSOB) was used to find out the effects of nodules and
scratches on wire bonds. The dimension of nodules including height, and the size of scratches including width were
measured prior to wire bonding. Wire bonding was then performed directly on various sizes of nodules and scratches on the
bonding pad, and the evaluation of wire bonds were conducted using wire pull tests before and after reliability test. Based on
the results of the wire bonding evaluation, the internal specification for nodules and scratches for wire bondable PCBs was
modified to allow nodules and scratches with a certain height and a width limitation, compared to initially adopted internal
specifications of no nodules and no scratches. Such an approach resulted in improved yield at the PCB manufacturer.
The development of chip-on-board (COB) type of image sensors has significantly increased in the last few years to
accommodate an increasing demand for low cost and high-performance industrial inspection cameras. Wire bonding is the
most commonly used technology for making the electrical interconnection between a silicon image sensor and its substrate
during image sensor fabrication. Therefore, wire bonding directly on the PCB surface is inevitable for COB type image
IPC-A-600J lists in section 22.214.171.124 Surface Plating – Wire Bond Pads that “Wire bond pads are free of surface nodules,
roughness, electrical test witness marks or scratches that exceed 0.8um (32uin) RMS (root-mean-square) in the pristine area
in accordance with an applicable test method AABUS.” Since the tolerance of surface nodules,
scratches. The average yield loss from multiple PCB products due to nodules and scratches for wire bonding boards were in
the range of 4% to 41% and 2% to 30%, respectively, during the period.
Figure 1 - Average Yield Loss from Multiple Wire Bonding PCB Products
It is worth to note that the data in Figure 1 may not necessarily provide the picture of actual average yield loss due to nodules
and scratches. When any defect, either nodule or scratch, was first found during inspection of a board, the reason for reject
was recorded, and further inspection of that board was not pursued since the board was already determined as a reject. For
example, the manufacturer recorded 39% of yield loss for nodules, and none for scratches in the period 3. However, it may
not mean that there were no scratches on those rejected boards since those boards had not been inspected further for scratches
after nodules were first observed.
Figure 2 shows the maximum yield loss for nodules and scratches. The maximum yield loss was recorded from one of the
PCB products that showed the lowest yield at the period or in the month. Unacceptable yield loss over the period of many
months initiated a discussion with the manufacturer in order to identify the root cause and conduct corrective actions to
improve on nodules and scratches.
Figure 2 – Maximum Yield Loss from a PCB Product with the Lowest Yield
Corrective Actions at the Manufacturer
The PCB Manufacturing Process
One of the PCB manufacturers who had experience producing the bare boards had considerable data that suggested that
nodules and scratches were likely the main reasons for yield loss. The specification initially defined by the user required
inspection at 20X starting magnification, which was beyond the IPC specification of 1.75X magnification. Since there were
inspection escapes, the manufacturer decided to start at 40X magnification as a preventative measure. This, combined with
the criteria for absolutely no nodules or any surface imperfection, resulted in many rejected boards, which may have actually
been wire bondable and reliable. The manufacturer initiated root cause analysis to determine the source of the nodules and
scratches in order to define an action plan to reduce or eliminate the defects.
Nodules are surface imperfections on the plated surface which can originate and grow in the copper plating process or
originate from processes preceding copper plating and grow in the copper plating process (i.e. electroless copper). Electroless
copper plating is used as a metallization process that deposits a thin layer of copper onto non-conductive surfaces, such as the
hole wall of a drilled panel. This creates electrical connectivity through the plated holes. Then, electrolytic copper plating
process uses an electrical current to electrodeposit copper from a copper sulfate solution onto the copper clad production
panel. Electroplating inherently prefers to plate onto protruding features, edges, or corners; therefore the slightest surface
protrusion on the base copper foil or a minor imperfection co-deposited during the electroless copper process will attract
more copper plating and grow in size to become a visually detectable nodule after electroplating.
Nodules that were observed optically under 40X magnification were cross sectioned in an attempt to determine the process at
which the nodule began to form. Given the small size of the nodules and knowing that the nodule starts with an even smaller
surface imperfection that grows through electroplating, cross sectioning down to the absolute center of the nodule was
difficult to achieve and objective evidence of the nodule’s origin could not be found all the time. Figure 3 shows an example
of a nodule cross-sectioned. In this case, it seemed to be clear that the nodule was formed prior to the Ni/Pd/Au plating
process, and, therefore, nodule formation would have likely happened during electroless or electrolytic copper plating.
Figure 3 – Cross-sectioned View of a Nodule as an Example
Using a fishbone diagram to define potential root causes of the nodules, a short list of potential root causes was identified:
copper foil imperfections, electroless copper co-deposited particles, and electroplated copper co-deposited particles. Each
potential root cause was explored in-depth to prove or disprove that it was the source of – or contributed to – the formation of
A random sample of copper foil was visually inspected under 100X magnification and no significant signs of imperfections
were found. Using a controlled production lot, a light mechanical scrubbing process was performed on the laminated foil
through a horizontal conveyorized machine, but the number of boards that were rejected for nodules remained close to the
average from previous production lots. Consequently, this potential root cause was eliminated early into the investigation.
The same mechanical scrubbing process was performed on panels that had been processed through electroless copper. In this
case, the results were noticeable. The density of nodule occurrences was reduced but there were still boards being rejected
for single nodules located at wire bond locations. And in some production lots, the frequency of the single nodules was
excessive enough to still have a significant impact on yield. However, an overall improvement had been made and this
mechanical scrubbing process became a standard process.
After an extended period of processing boards with the mechanical scrubbing process after electroless copper, an opportunity
to test the electrolytic copper plating process arose when an annual preventative maintenance procedure was completed on
one of the three plating tanks on the automated plating line. The procedure